Do you need custom fasteners created with Titanium? Since our inception, Vegas Fastener Group has met every challenge of providing Quality, Timely, Cost-effective solutions for specialty fastener applications. Every product is built to your specifications, using your prints if necessary.
Below are the technical specifications of the Titanium Bar Stock we have available to meet your needs.
Subcategory: Metal; Nonferrous Metal; Pure Metallic Element; Titanium Alloy Close Analogs: A wide range of Ti alloys are listed in MatWeb. Titanium Grades 1,2,3,4,7,11,and 12 are all considered unalloyed. This listing is for ‘pure’ titanium. Key Words: biomaterials, biomedical implants, biocompatibility
Material Notes: This listing is for ‘pure’ titanium. Although unalloyed titanium is not very useful for structural applications, titanium alloys are highly praised for their use in aerospace, high-temperature and biomedical applications. Titanium is difficult to machine or weld, but has significant advantages over traditional metals. For medical implants, titanium is considered one of the most biocompatible materials available, especially where direct contact to tissue or bone is required (i.e. endosseuos dental implants or porous uncemented orthopedic implants). See the individual titanium alloy datasheets for specific applications.
|Density||4.5 g/cc||0.163 lb/in³|
|Hardness, Brinell||70||70||electrolytic Ti|
|Tensile Strength, Ultimate||220 MPa||31900 psi|
|Tensile Strength, Yield||140 MPa||20300 psi|
|Elongation at Break||54 %||54 %|
|Modulus of Elasticity||116 GPa||16800 ksi|
|Electrical Resistivity||5.54e-005 ohm-cm||5.54e-005 ohm-cm|
|Critical Magnetic Field Strength, Oersted||56||56|
|Critical Superconducting Temperature||0.36 – 0.44 K||0.36 – 0.44 K|
|Heat of Fusion||435.4 J/g||187 BTU/lb|
|CTE, linear 20°C||8.9 µm/m-°C||4.94 µin/in-°F||over the range 20-100ºC|
|CTE, linear 1000°C||10.1 µm/m-°C||5.61 µin/in-°F|
|Heat Capacity||0.528 J/g-°C||0.126 BTU/lb-°F|
|Thermal Conductivity||17 W/m-K||118 BTU-in/hr-ft²-°F|
|Melting Point||1650 – 1670 °C||3000 – 3040 °F|
|Emissivity (0-1)||0.63||0.63||unoxidized; 650 nm|
References are available for this material.